- Research article
- Open Access
- Open Peer Review
An ex vivo continuous passive motion model in a porcine knee for assessing primary stability of cell-free collagen gel plugs
© Efe et al; licensee BioMed Central Ltd. 2010
- Received: 2 August 2010
- Accepted: 15 December 2010
- Published: 15 December 2010
Primary stability of cartilage repair constructs is of the utmost importance in the clinical setting but few continuous passive motion (CPM) models are available. Our study aimed to establish a novel ex vivo CPM animal model and to evaluate the required motion cycles for testing the mechanical properties of a new cell-free collagen type I gel plug (CaReS®-1S).
A novel ex vivo CPM device was developed. Full-thickness cartilage defects (11 mm diameter by 6 mm deep) were created on the medial femoral condyle of porcine knee specimens. CaReS®-1S was implanted in 16 animals and each knee underwent continuous passive motion. After 0, 2000, 4000, 6000, and 8000 motions, standardized digital pictures of the grafts were taken, focusing on the worn surfaces. The percentage of worn surface on the total CaReS®-1S surface was evaluated with image processing software.
Significant differences in the worn surface were recorded between 0 and 2000 motion cycles (p < 0.0001). After 2000 motion cycles, there was no significant difference. No total delamination of CaReS®-1S with an empty defect site was recorded.
The ex vivo CPM animal model is appropriate in investigating CaReS®-1S durability under continuous passive motion. 2000 motion cycles appear adequate to assess the primary stability of type I collagen gels used to repair focal chondral defects.
- Wear Surface
- Cartilage Defect
- Mechanical Axis
- Primary Stability
- Continuous Passive Motion
Cartilage defects of the knee are commonly encountered in orthopedic clinical practice [1, 2]. Several well described repair strategies have been used in the management of chondral lesions [3–6]. Debate persists about the best repair technique for symptomatic chondral defects of less than 2 cm² . Currently, CaReS®-1S (Arthro Kinetics, Esslingen, Germany), a cell-free collagen type I gel plug was introduced to treat isolated cartilage defects. This graft is implanted in the debrided chondral lesion, in a single-stage procedure. The gel triggers chondrocyte migration and proliferation into the plug, which has been proven both in vitro and ex vivo .
Most cartilage regenerative studies address the biochemical and histological composition of generated cartilage [9, 10]. However, successful cartilage repair requires sufficient initial mechanical stability of the grafts . The implanted grafts should withstand the forces in vivo in the early postoperative phase during joint movement. Secure primary stability is necessary to keep the grafts in place and to achieve sufficient joint surface congruity, on which the long-term results depend . Partially or completely delaminated tissue engineered constructs can cause locking in the knee and poor clinical results [13, 14].
Several authors describe the beneficial effects of continuous passive motion (CPM) on neochondrogenesis and most postoperative protocols consider ex vivo non-weight bearing CPM in the first 6 weeks after surgery to be beneficial [15–17].
Drobnic et al.  reported a human cadaveric model of ex vivo CPM, testing four fixation techniques for fibrinogen and thrombin coated collagen fleece. They aimed to simulate the initial postoperative period by applying ex vivo CPM to specimens. However, the availability of appropriate human specimens without advanced osteoarthritis is limited. This can be a challenge for developing appropriate protocols to test the primary stability of collagen plugs; to date, there are no established animal models.
Moreover, little is known about the required motion cycles for testing the mechanical properties of cartilage repair constructs. The means to assess the early postoperative phase after cartilage regenerative procedures is lacking. Consequently, efforts to build a new ex vivo CPM device to assess the mechanical properties of tissue engineered scaffolds would be of great value. The aim of the present study is to construct a simplified, custom-made ex vivo CPM device and to investigate the number of motion cycles required for testing the mechanical properties of collagen plugs. We hypothesized that the new device would allow us to reliably evaluate the degree of wear to collagen plugs. We also aimed to determine the number of cycles required to assess wear appropriately using this model.
Sixteen porcine knees (age 9 months) were used to assess primary stability of cell-free collagen gel plugs. These were obtained from the local butcher, fresh frozen at -25°, and thawed for 16 hours at room temperature (20°C) before testing. This project was performed in accordance with the Helsinki Declaration and with local legislation. CaReS®-1S was implanted in an identical manner in each specimen. Right and left knees were not differentiated; both knees were used . Some knee specimens were dissected to evaluate the anatomy of the porcine knee and to establish the surgical procedure.
CaReS®-1S is a sterile cylindrical, three-dimensional collagen-based and cell-free gel plug, consisting of 4.8 mg/mL rat tail collagen type I (CaReS®[20, 21], Arthro Kinetics, Esslingen, Germany). It has been used for cartilage defects in the knee and ankle in patients under 50 years of age. The plug is available in three different diameters (11, 22, and 34 mm) and thicknesses (4, 6, and 8 mm). The hydrogel consistency allows adequate coverage and sufficient reconstruction of the articular surface. The basic concept of CaReS®-1S is to replenish the cartilage defect with a matrix structure, facilitating autologous chondrocytes to penetrate into the lesion zone. Low antigenicity and high biocompatibility of CaReS®-1S is achieved by the high conservation of protein sequences of collagen type I within various species. The plugs used in this study measured 11 mm diameter by 6 mm deep and contained 4.27 mg collagen type I. CaReS®-1S were stored in phosphate-buffered saline solution and preserved at 4°C until use.
Ex vivo CPM device
The tibia and the femur were transected approximately 10 cm proximal and distal to the knee joint, preserving muscles, articular capsule, ligaments, and tendons. A medial parapatellar arthrotomy was performed and the patella was dislocated laterally. A standardized full-thickness cartilage defect of 11 mm diameter by 6 mm deep was created in the weight-bearing area of the medial femoral condyle using a punch (Arthro Kinetics, Esslingen, Germany).
Ex vivo CPM protocol
The repeated measured data at 2000, 4000, 6000, and 8000 motion cycles were assessed by analysis of variance (ANOVA). The increase in the worn surface within the first 2000 motion cycles and differences between 2000, 4000, 6000, and 8000 motion cycles were analyzed through the application of general linear hypothesis testing. P-value adjustment was performed by the method of Shaffer . Additionally, for all contrasts, the corresponding 95% family-wise confidence intervals (CI) were calculated. Two-sided adjusted p-values less than 0.05 were considered statistically significant. All statistical analysis was performed with R software (Foundation for Statistical Computing, Vienna, Austria).
Analysis of surface wear in dependence of motion cycles (p < 0.05)
Mean difference of worn surface (%)
95% Confidence Interval
0 to 2000
10.2 - 30.2
2000 to 4000
-1.5 - 5.3
2000 to 6000
-0.6 - 6.3
2000 to 8000
-1.1 - 5.7
Information on ex vivo CPM devices and the number of motion cycles needed to investigate cartilage repair constructs is lacking. The aim of our study was to construct a novel ex vivo CPM device and to create a small animal model to evaluate the required number of continuous passive motions for testing CaReS®-1S. Our hypothesis that this device would allow reproducible evaluation of wear to collagen plugs was proven to be correct. We also successfully determined number of cycles required to assess wear appropriately.
There are several limitations to our study. While porcine anatomy closely approximates human anatomy , immanent differences between species are evident. Mechanical in vitro studies only simulate the physiological function and motion of the joint, since there is no force applied by the muscles. The presented ex vivo CPM device may only partially simulate its clinical application. In our study, analysis of the worn surface of the graft was performed by imaging processing software as a semiquantitative analysis. More objective quantitative measurements and absolute values may be preferable. However, analysis of cartilage repair constructs with the ex vivo CPM is difficult, raising the question of reliability. Other studies used qualitative scales [18, 24], posing the problem of subjective bias. It is very likely that a potential malalignment of the joint within the testing device may have affected the results. In our setup, the tibia was allowed to rotate freely. It was also allowed to move freely in the frontal plane. Malalignment in the testing device resulted in impingement of the specimen with the frame. Simulation in human cadaver knees would be the optimal standard for testing. However, human specimens are expensive, sometimes difficult to obtain, and come from elderly people. Therefore, osteoarthritic changes are a common finding in these specimens, which may interfere with the evaluation of a procedure in an otherwise healthy joint of a young patient. The porcine model comes with the advantage of unlimited availability at a low cost.
There are currently only two experimental ex vivo CPM models for testing cartilage implants. A recent study on human cadaver knees investigated the quality of PEOT/PBT scaffold fixation (transosseous fixation, fibrin glue, biodegradable pins, and continuous cartilage sutures) by ex vivo CPM in a vertical position . The mechanical behavior was evaluated after 60 and 150 motion cycles with a 35N load, focusing on outline attachment, scaffold integrity, and area coverage. After 210 motion cycles, an endpoint fixation test was performed. Drobnic et al. compared in a similar model four different fixation techniques (self-adhesion, fibrin glue, bone sutures, periosteal cover) of a collagen scaffold in the human cadaveric knee, horizontally oriented with and without loading. In both studies, the numbers of cycles remained small and did not correspond with the clinical situation after surgical management of cartilage defects; whereas ex vivo CPM is often applied several hours a day. It is most likely that in the early postoperative phase the knee undergoes considerably more than 150 motion cycles. At our institution and in previous experience  patients usually use the ex vivo CPM machine for 6 to 8 hours daily after implantation of tissue engineered constructs. The rate is one cycle per minute but varies based on patient comfort and performance. This fact should be taken into consideration when performing mechanical testing. A study design with fewer motion cycles makes the transformation from in vitro to in vivo testing difficult. Consequently, long-term durability studies are necessary. However, it is possible to determine if such constructs were too fragile to be practical. Thus, shorter-term motion cycles studies have their place. In the present study, testing of CaReS®-1S was performed with 8000 motion cycles under ex vivo CPM. The question of how many motion cycles were necessary to evaluate wear to collagen plugs has not been answered satisfactorily as of yet. In our study, significant changes in the worn surface of the graft were only detected between 0 and 2000 motion cycles (p = 0.0001). Therefore, a protocol with 2000 motion cycles appears to be a sufficient number to investigate type I collagen gels used to repair focal chondral defects.
Delamination of tissue engineered constructs occurs mainly in the first six postoperative months. A possible explanation for this may include weak mechanical fixation and adherence. Since it is known that friction forces and shear forces may cause delamination of cartilage implants , most authors allow only partial weight-bearing after cartilage regeneration techniques [28, 29]. While Drobnic et al.  and Bekkers et al.  used additional load ex vivo CPM protocols, intraarticular pressure measurements were not performed. It remains unclear how much load was applied on the specimens intraarticularly. Although no additional load was applied in our study, we assume that the vertical orientation, the corresponding tibial cartilage, and the intraarticular liquid generates friction forces and shear forces on the gel that correspond with the clinical setting. Nevertheless, performing the experiments with an additional load might have been preferable.
Evaluation of tissue engineered constructs in the early postoperative rehabilitation phase is difficult. The ex vivo CPM device used in the present study is simplified and can be helpful to investigate the durability of collagen gel constructs. Our findings may support research in new materials in a porcine knee model. Nevertheless, the ex vivo CPM device cannot be used in assessing biomechanical properties (viscoelasticity, permeability, tensile strength, and electromechanical properties).
The novel custom-made ex vivo CPM device allows the investigation of CaReS®-1S under a high number of motion cycles. Significant differences in the worn surface were detected between 0 and 2000 motion cycles, but not beyond 2000 cycles. This device and study model may be of great value in further investigations.
The authors wish to thank Dr. Karsten Gavenis, Department of Orthopaedic Surgery, University Hospital Aachen, Germany, and Professor Ulrich Schneider, Arthro Nova Clinic, Tegernsee, Germany for providing the laboratory facilities.
- Curl WW, Krome J, Gordon ES, Rushing J, Smith BP, Poehling GG: Cartilage injuries: a review of 31,516 knee arthroscopies. Arthroscopy. 1997, 13 (4): 456-460. 10.1016/S0749-8063(97)90124-9.View ArticlePubMedGoogle Scholar
- Hjelle K, Solheim E, Strand T, Muri R, Brittberg M: Articular cartilage defects in 1,000 knee arthroscopies. Arthroscopy. 2002, 18 (7): 730-734. 10.1053/jars.2002.32839.View ArticlePubMedGoogle Scholar
- Bert JM, Maschka K: The arthroscopic treatment of unicompartmental gonarthrosis: a five-year follow-up study of abrasion arthroplasty plus arthroscopic debridement and arthroscopic debridement alone. Arthroscopy. 1989, 5 (1): 25-32. 10.1016/0749-8063(89)90086-8.View ArticlePubMedGoogle Scholar
- Hangody L, Vasarhelyi G, Hangody LR, Sukosd Z, Tibay G, Bartha L, Bodo G: Autologous osteochondral grafting--technique and long-term results. Injury. 2008, 39 (Suppl 1): S32-39. 10.1016/j.injury.2008.01.041.View ArticlePubMedGoogle Scholar
- Mithoefer K, Williams RJ, Warren RF, Potter HG, Spock CR, Jones EC, Wickiewicz TL, Marx RG: The microfracture technique for the treatment of articular cartilage lesions in the knee. A prospective cohort study. J Bone Joint Surg Am. 2005, 87 (9): 1911-1920. 10.2106/JBJS.D.02846.View ArticlePubMedGoogle Scholar
- Rae PJ, Noble J: Arthroscopic drilling of osteochondral lesions of the knee. J Bone Joint Surg Br. 1989, 71 (3): 534-PubMedGoogle Scholar
- Smith GD, Knutsen G, Richardson JB: A clinical review of cartilage repair techniques. J Bone Joint Surg Br. 2005, 87 (4): 445-449. 10.1302/0301-620X.87B4.15971.View ArticlePubMedGoogle Scholar
- Morales TI: Chondrocyte moves: clever strategies?. Osteoarthritis Cartilage. 2007, 15 (8): 861-871. 10.1016/j.joca.2007.02.022.View ArticlePubMedPubMed CentralGoogle Scholar
- Getgood A, Brooks R, Fortier L, Rushton N: Articular cartilage tissue engineering: today's research, tomorrow's practice?. J Bone Joint Surg Br. 2009, 91 (5): 565-576. 10.1302/0301-620X.91B5.21832.View ArticlePubMedGoogle Scholar
- van Osch GJ, Brittberg M, Dennis JE, Bastiaansen-Jenniskens YM, Erben RG, Konttinen YT, Luyten FP: Cartilage repair: past and future--lessons for regenerative medicine. J Cell Mol Med. 2009, 13 (5): 792-810. 10.1111/j.1582-4934.2009.00789.x.View ArticlePubMedPubMed CentralGoogle Scholar
- Sittinger M, Hutmacher DW, Risbud MV: Current strategies for cell delivery in cartilage and bone regeneration. Curr Opin Biotechnol. 2004, 15 (5): 411-418. 10.1016/j.copbio.2004.08.010.View ArticlePubMedGoogle Scholar
- Sittinger M, Perka C, Schultz O, Haupl T, Burmester GR: Joint cartilage regeneration by tissue engineering. Z Rheumatol. 1999, 58 (3): 130-135. 10.1007/s003930050162.View ArticlePubMedGoogle Scholar
- Nehrer S, Spector M, Minas T: Histologic analysis of tissue after failed cartilage repair procedures. Clin Orthop Relat Res. 1999, 149-162. 10.1097/00003086-199908000-00020. 365Google Scholar
- Peterson L, Minas T, Brittberg M, Nilsson A, Sjogren-Jansson E, Lindahl A: Two- to 9-year outcome after autologous chondrocyte transplantation of the knee. Clin Orthop Relat Res. 2000, 212-234. 10.1097/00003086-200005000-00020. 374Google Scholar
- Gikas PD, Bayliss L, Bentley G, Briggs TW: An overview of autologous chondrocyte implantation. J Bone Joint Surg Br. 2009, 91 (8): 997-1006. 10.1302/0301-620X.91B8.21824.View ArticlePubMedGoogle Scholar
- Moran ME, Kim HK, Salter RB: Biological resurfacing of full-thickness defects in patellar articular cartilage of the rabbit. Investigation of autogenous periosteal grafts subjected to continuous passive motion. J Bone Joint Surg Br. 1992, 74 (5): 659-667.PubMedGoogle Scholar
- O'Driscoll SW, Keeley FW, Salter RB: The chondrogenic potential of free autogenous periosteal grafts for biological resurfacing of major full-thickness defects in joint surfaces under the influence of continuous passive motion. An experimental investigation in the rabbit. J Bone Joint Surg Am. 1986, 68 (7): 1017-1035.PubMedGoogle Scholar
- Drobnic M, Radosavljevic D, Ravnik D, Pavlovcic V, Hribernik M: Comparison of four techniques for the fixation of a collagen scaffold in the human cadaveric knee. Osteoarthritis Cartilage. 2006, 14 (4): 337-344. 10.1016/j.joca.2005.11.007.View ArticlePubMedGoogle Scholar
- Athanasiou KA, Rosenwasser MP, Buckwalter JA, Malinin TI, Mow VC: Interspecies comparisons of in situ intrinsic mechanical properties of distal femoral cartilage. J Orthop Res. 1991, 9 (3): 330-340. 10.1002/jor.1100090304.View ArticlePubMedGoogle Scholar
- Andereya S, Maus U, Gavenis K, Muller-Rath R, Miltner O, Mumme T, Schneider U: [First clinical experiences with a novel 3D-collagen gel (CaReS) for the treatment of focal cartilage defects in the knee]. Z Orthop Ihre Grenzgeb. 2006, 144 (3): 272-280. 10.1055/s-2006-933445.View ArticlePubMedGoogle Scholar
- Schneider U, Andereya S: [First results of a prospective randomized clinical trial on traditional chondrocyte transplantation vs CaReS-Technology]. Z Orthop Ihre Grenzgeb. 2003, 141 (5): 496-497.PubMedGoogle Scholar
- Shaffer J: Modified sequentially rejective multiple test procedures. Journal of the American Statistical Association. 1986, 81: 826-831. 10.2307/2289016.View ArticleGoogle Scholar
- Ahern BJ, Parvizi J, Boston R, Schaer TP: Preclinical animal models in single site cartilage defect testing: a systematic review. Osteoarthritis Cartilage. 2009, 17 (6): 705-713. 10.1016/j.joca.2008.11.008.View ArticlePubMedGoogle Scholar
- Bekkers JE, Tsuchida AI, Malda J, Creemers LB, Castelein RJ, Saris DB, Dhert WJ: Quality of scaffold fixation in a human cadaver knee model. Osteoarthritis Cartilage. 18 (2): 266-272. 10.1016/j.joca.2009.09.001.Google Scholar
- Alford JW, Cole BJ: Cartilage restoration, part 2: techniques, outcomes, and future directions. Am J Sports Med. 2005, 33 (3): 443-460. 10.1177/0363546505274578.View ArticlePubMedGoogle Scholar
- Alparslan L, Minas T, Winalski CS: Magnetic resonance imaging of autologous chondrocyte implantation. Semin Ultrasound CT MR. 2001, 22 (4): 341-351. 10.1016/S0887-2171(01)90025-3.View ArticlePubMedGoogle Scholar
- Driesang IM, Hunziker EB: Delamination rates of tissue flaps used in articular cartilage repair. J Orthop Res. 2000, 18 (6): 909-911. 10.1002/jor.1100180609.View ArticlePubMedGoogle Scholar
- Marcacci M, Zaffagnini S, Kon E, Visani A, Iacono F, Loreti I: Arthroscopic autologous chondrocyte transplantation: technical note. Knee Surg Sports Traumatol Arthrosc. 2002, 10 (3): 154-159. 10.1007/s00167-001-0275-6.View ArticlePubMedGoogle Scholar
- Peterson L, Brittberg M, Kiviranta I, Akerlund EL, Lindahl A: Autologous chondrocyte transplantation. Biomechanics and long-term durability. Am J Sports Med. 2002, 30 (1): 2-12.PubMedGoogle Scholar
- The pre-publication history for this paper can be accessed here:http://www.biomedcentral.com/1471-2474/11/283/prepub
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (<url>http://creativecommons.org/licenses/by/2.0</url>), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.